Dent Clin N Am 51 (2007) 333–357 New Developments in Dental Adhesion Jorge Perdigao, DMD, MS, PhD ˜ Division of Operative Dentistry, Department of Restorative Sciences, University of Minnesota, 8-450 Moos Health Sciences Tower, 515 Delaware Street SE, Minneapolis, MN 55455, USA Adhesion or bonding is the process of forming an adhesive joint, whichconsists of two substrates joined together. In dentistry, the adherend is thesubstrate to which the adhesivedenamel and dentin, rarely cementumdis applied. Dental adhesives are solutions of resin monomers that join arestorative material with a dental substrate after the monomers set by poly-merization. While most adhesive joints involve only two interfaces, dentaladhesive joints may be more complex such as the enamel–adhesive–compos-ite–adhesive–porcelain interface formed when a clinician bonds a porcelainrestoration (Fig. 1). A bonded composite restoration is another example ofa complex adhesive joint. In 1955, Buonocore  reported the use of 85% phosphoric acid toimprove the retention of an acrylic resin on enamel. The micromechanicalnature of the interaction of dental adhesives with enamel is a result of theinﬁltration of resin monomers into the microporosities left by the aciddissolution of enamel and subsequent enveloping of the exposed hydroxyap-atite crystals with the polymerized monomers within the pores on theenamel surface . The ultimate goal of a bonded restoration is to attain an intimate adap-tation of the restorative material with the dental substrate . This task isdiﬃcult to achieve as the bonding process for enamel is diﬀerent fromthat for dentin. That is, dentin is more humid and more organic than enamel. While enamel is composed of 96% hydroxyapatite (mineral) by weight,dentin contains a signiﬁcant amount of water and organic material, mainlytype-I collagen . This humid and organic nature of dentin makes bondingto this hard tissue extremely diﬃcult. When tooth structure is cut with a bur or other instrument, the residualcomponents form a ‘‘smear layer’’ of debris on the surface . This debris E-mail address: firstname.lastname@example.org/07/$ - see front matter Ó 2007 Elsevier Inc. All rights reserved.doi:10.1016/j.cden.2007.01.001 dental.theclinics.com
334 ˜ PERDIGAO Porcelain etched with HF Silane Dental adhesive Composite (resin cement) Dental adhesive Etched enamelFig. 1. Adhesive joint formed between enamel and etched porcelain. HF, hydroﬂuoric acid.forms a uniform coating on enamel and dentin and plugs the entrance of thedentinal tubules, reducing the permeability of dentin (Fig. 2). The smearlayer is porous and permeable as a result of submicron channels that allowthe dentinal ﬂuid to pass through . The basic composition of the smearlayer is hydroxyapatite and altered collagen with an external surface formedby gellike denatured collagen . The morphology of the smear layer is de-termined to a large extent by the type of instrument that creates it and by thesite of dentin where it is formed [8,9]. Fig. 2. Field emission scanning electron micrograph of dentin smear layer and smear plug.
DENTAL ADHESION 335 As the smear layer constitutes a true physical barrier, it must be dis-solved or made permeable so the monomers in the adhesives can contactthe dentin surface directly. In spite of diﬀerent classiﬁcations of adhesivesystems, the current adhesion strategies depend exclusively on how dentaladhesives interact with this smear layer. One strategy involves etch-and-rinse adhesives, which remove the smear layer and superﬁcial hydroxyapa-tite through etching with a separate acid gel (Fig. 3). The second strategyinvolves self-etch adhesives, which make the smear layer permeable withoutremoving it completely (Figs. 4 and 5). Fig. 6 summarizes the current bond-ing strategies.Etch-and-rinse strategy With the etch-and-rinse strategy, dentin and enamel are treated with anacid gel (commonly phosphoric acid) to remove the smear layer and demin-eralize the most superﬁcial hydroxyapatite crystals (Fig. 7). Following thischemical etching, a mixture of resin monomers (primer/adhesive) dissolvedin an organic solvent is applied to inﬁltrate etched dentin . The resinmonomers permeate the water-ﬁlled spaces between adjacent dentin colla-gen ﬁbers that used to be occupied by hydroxyapatite crystals. This inﬁltra-tion results in a hybrid tissue composed of collagen, resin, residualhydroxyapatite, and traces of water (see Fig. 3) known as the resin–dentininterdiﬀusion zone, ﬁrst described in 1982 as the hybrid layer . This in-timate micromechanical entanglement of resin monomers with etched dentin Fig. 3. Interaction of one-bottle etch-and-rinse adhesives with dentin.
336 ˜ PERDIGAO Fig. 4. Interaction of two-bottle self-etch adhesives with dentin.may result in decreased postoperative sensitivity, may make for a bettermarginal ﬁt, and may even act as an elastic buﬀer that compensates forthe polymerization shrinkage stress during contraction of the restorativecomposite [12–14]. Fig. 5. Interaction of all-in-one self-etch adhesives with dentin.
DENTAL ADHESION 337 Fig. 6. Summary of current adhesion strategies.Self-etch strategy The latest development in dental adhesion is based on simpliﬁcation andreduced application time. These self-etch (nonrinsing) adhesives do notrequire a separate acid-etch step as they condition and prime enamel anddentin simultaneously by inﬁltrating and partially dissolving the smear layerFig. 7. Field emission scanning electron micrograph of dentin etched with 40% phosphoric acidfor 15 seconds. Note the collagen ﬁbers deprived from hydroxyapatite crystals as a result of aciddemineralization. The more intense decalciﬁcation around the peritubular area may be a resultof both the high mineral content of the peritubular region and the easier penetration of the acidthrough the tubular lumen.
338 ˜ PERDIGAOand hydroxyapatite to generate a hybrid zone that incorporates mineralsand the smear layer . The ﬁrst self-etch nonrinsing adhesives were composed of two solutions, anacidic primer and a bonding resin (see Fig. 4). Recently, many clinicians haveshifted to one-step self-etch systems (also named all-in-one adhesives) inwhich manufacturers have attempted to incorporate all the primary compo-nents of an adhesive system (etchant, primer, and bonding resin) into a singlesolution (see Fig. 5). Both the acidic primer of two-step self-etch adhesives andthe all-in-one solution are composed of aqueous mixtures of acidic functionalmonomers, generally phosphoric-acid or carboxylic-acid esters, with a pHhigher than that of phosphoric acid gels . Water is an essential componentof self-etch adhesives as it participates in the ionization of the acidic moieties. All-in-one adhesives are user-friendly in that fewer steps are required forthe bonding protocol. The elimination of separate etching and rinsing stepssimpliﬁed the bonding technique, making these systems more popular indaily practice . Self-etch adhesives diﬀer in their aggressiveness. Therefore they are clas-siﬁed in three categories according to acidity: mild, moderate, and aggressive[16,18]. Because self-etch adhesives are not as aggressive as the phosphoric-acid gel in etch-and-rinse adhesives, most do not remove the smear layer(Fig. 8). Adper Prompt L-Pop (3M ESPE) is considered an aggressiveself-etch adhesive (pH ¼ 0.9–1.0), while other all-in-one adhesives, such as-Clearﬁl S3 Bond, iBond, and G-Bond, are mild or moderate (pH O1.5)(Table 1) [19–22].Enamel bonding with self-etch adhesives The enamel bond strengths of the earliest self-etch adhesives were lowerthan those associated with adhesives that rely on a separate etching step .Fig. 8. Field emission scanning electron micrograph of a resin–dentin interface formed withClearﬁl S3 Bond (Kuraray). The neck of the resin tag contains residual smear layer particles.Ad, adhesive; D, dentin; RT, resin tag; SP, resin-impregnated smear plug.
DENTAL ADHESION 339Table 1pHa of self-etch adhesivesAdhesive (manufacturer) pHAdheSE (Ivoclar Vivadent) 1.7Adper Prompt L-Pop (3M ESPE) 0.9–1.0Clearﬁl S3 Bond (Kuraray) 2.4Clearﬁl SE Bond (Kuraray) 1.8iBond (Heraeus Kulzer) 2.2Xeno IV (Dentsply Caulk) 2.5 a pH of 35% silica-thickened phosphoric-acid gel ¼ 0–0.4. Data from Refs. [19–22].Because of their higher pH, two-step self-etch adhesives result in shallowerenamel demineralization compared with that of phosphoric acid [16,23].Nevertheless, roughening of enamel to remove prismless enamel improvesthe enamel-bonding ability of self-etch adhesives . A separate phospho-ric-acid enamel-etching step also enhances the eﬃcacy of self-etch adhesives. Two-step self-etch adhesives bond at an acceptable level to normal den-tin and to ground enamel in vitro [26–28]. Conversely, two-step self-etchmaterials may not bond as well to intact enamel and sclerotic dentin[16,24,29,30]. All-in-one self-etch systems are not as acidic as the phosphoric acid usedwith the etch-and-rinse adhesives . This characteristic has raised concernsabout the performance of all-in-one self-etch systems on intact enamel(Fig. 9). Several in vitro investigations have reported low resin–enamelbond strength of all-in-one self-etch materials [15,26,30,31]. Grinding theenamel during a bevel or cavity preparation, for instance, makes the sub-strate more receptive for bonding with all-in-one self-etch systems [31,32].Fig. 9. Backscattered ﬁeld emission scanning electron micrograph of resin–enamel interfaceformed by Xeno IV (Dentsply). The restorative material used was Filtek Z250 (3M ESPE).Intense silver deposits at the resin–enamel interface (asterisks) denote intense enamel leakage.Ad, adhesive; Comp, composite restoration.
340 ˜ PERDIGAO Despite the increased popularity of self-etch adhesives, etching with phos-phoric acid is still considered the golden standard against which new mate-rials are tested .Dentin bonding with self-etch adhesives In spite of their user-friendliness and low technique sensitivity, all-in-oneadhesives have resulted in low bonding eﬀectiveness in vitro [15,26,30] whiletheir clinical reliability has often been questioned. Another drawback asso-ciated with all-in-one adhesives is their behavior as semipermeable mem-branes. These materials allow the movement of water across the bondedinterface, which potentially leads to hydrolytic degradation (Fig. 10) [31,32]. Consistent information regarding the durability of self-etch adhesiveswhen applied on dentin is available in the literature [28,33,34]. Althoughhigh early resin–dentin bond-strength values may be achieved with self-etch adhesives, their bonding eﬀectiveness over time is disappointing[28,33,34]. Because of the high hydrophilic nature of the acidic monomersand the high water concentration required for ionization of the acidic mono-mers in all-in-one self-etch solutions, these materials are likely to have resin–enamel bonds compromised over time. An inadequate resin penetration intotooth substrates may result in accelerated degradation of the structure of thebonding interface . As polymerization shrinkage stresses the bonding in-terface, dentin adhesives that do not resist these stresses result in low bondstrengths, marginal gaps, recurrent caries, and pulpal irritation [33,35]. For some all-in-one adhesives, performance may depend on the applica-tion method, as the number of coats recommended by the manufacturermay not suﬃce [30,36]. All-in-one adhesives have resulted in a wide rangeof dentin bond strengths [30,36,37]. Application of the all-in-one adhesivein multiple layers may result in higher bond strengths [37,38] and betterFig. 10. Transmission electron micrograph of resin–dentin interface formed with Clearﬁl S3Bond (Kuraray). Deposits of silver grains may correspond to areas of residual water. D, dentin;H, hybrid layer.
DENTAL ADHESION 341inﬁltration into the hybrid layer . One manufacturer recommends rub-bing the adhesive continuously for 15 seconds, followed by the applicationof a second coat after gentle air-drying and curing the ﬁrst coat. This secondcoat prevents the formation of dry spots on the dentin surface and mayresult in better impregnation of the monomers into the hybrid layer, asobserved in Figs. 11 and 12. Low enamel and dentin bond strengths have been reported when acetone-based all-in-one adhesives are applied as per manufacturer’s directions[33,37]. These adhesives result in severe enamel microleakage following ther-mal stresses [39,40]. When applied to one-surface occlusal preparations, oneof the most popular acetone-based all-in-one adhesives is not able to with-stand polymerization shrinkage stresses nor thermocycling, resulting ina high percentage of pretesting debonds . Several mechanisms may ac-count for this poor performance as compared with adhesives with diﬀerentsolvents. The magnitude of dentin bond strengths depends on the degreeof inﬁltration of the resin monomers into the collagen pretreated with anacidic conditioner or with phosphoric acid . The author’s electron mi-croscopy analyses (Figs. 13 and 14) have demonstrated that acetone-basedall-in-one adhesives result in a hybrid layer 0.2 to 0.5 mm thick, interfacialgaps, and limited resin penetration into the dentinal tubules. It is knownthat hybrid layers are particularly susceptible to degradation when thecavo-surface margins are not in enamel . The degradation of the dentinbonding interface is caused by the availability of exposed collagen ﬁbrils atthe base of hybrid layer  or by hydrolytic degradation of resin compo-nents in the hybrid layer [28,43–45]. Water can also inﬁltrate and plasticizeFig. 11. Field emission scanning electron micrograph of the dentin hybridization formed uponapplication of two coats of Adper Prompt L-Pop. Note the inﬁltration of the material into thedentin tubules and the absence of interfacial gaps. When Adper Prompt L-Pop is applied in onecoat, a separation gap forms between the adhesive and the hybrid layer (not shown). Ad, adhe-sive; Comp, composite restoration; D, dentin; H, hybrid layer.
342 ˜ PERDIGAOFig. 12. Transmission electron micrograph of the dentin hybridization formed upon appli-cation of two coats of Adper Prompt L-Pop (3M ESPE). Note the reticular morphology ofthe hybrid layer corresponding to the resin embedding of the collagen ﬁbers. Ad, adhesive;C, composite particle; D, dentin; H, hybrid layer.the resin matrix, which decreases the mechanical properties of the polymer. Other factors may play a role in the weak bonding performance of ace-tone-containing all-in-one adhesives. Porosities (or blisters) occur at theenamel and dentin bonding interfaces because most all-in-one adhesivesbehave as semipermeable membranes [31,33,47–49]. These porosities maybe a result of water accumulation either caused by an osmotic gradient orby monomer–solvent phase separation upon evaporation of the acetone[21,49]. The number and size of these blisters may also depend on the inten-sity of the air-drying step . High hydrophilicity, and consequent higher water sorption, has been re-ported associated with another acetone-based all-in-one adhesive containingFig. 13. Field emission scanning electron micrograph of a resin–dentin interface formed withG-Bond (GC America). Ad, adhesive; Comp, composite restoration; D, dentin.
DENTAL ADHESION 343Fig. 14. Transmission electron micrograph of a resin–dentin interface formed with G-Bond(GC America) Asterisks indicate residual smear particles. Ad, adhesive; D, dentin; H, hybridlayer; SP, smear plug; T, resin tag.a poly-phosphate molecule, dipentaerythritol penta-acrylate phosphate .The adhesive may undergo a substantial reduction in elastic modulus afterwater sorption, due to the plasticizing eﬀect of water . If the adhesivehas been plasticized by water, the restoration will likely fail when a loadis applied on the surface because the stresses cannot be transferred acrossthe adhesive joint. Another factor that may lead to lower bond strengthsis the adhesive’s low degree of conversion, which has been demonstratedfor speciﬁc adhesive compositions . Clearﬁl SE Bond (Kuraray) (Table 2), a two-step self-etch adhesive basedon 10-methacryloyloxy decyl dihydrogen phosphate (10-MDP), is a refer-ence for all other self-etch adhesives when it comes to dentin bond strengths[15,28]. In the author’s laboratory, Clearﬁl S3 Bond, the all-in-one successorof Clearﬁl SE Bond, shows lower dentin bond strengths than its predecessor.The pH of Clearﬁl S3 Bond is less acidic than that of Clearﬁl SE Bondprimer (2.4 versus 1.8, respectively). In spite of its relatively high pH, thebond strengths of Clearﬁl S3 Bond on unground enamel are statistically sim-ilar to those of a more aggressive self-etch adhesive, Adper Prompt L-Pop(pH ¼ 0.9–1.0) when tested in the author’s laboratory. The manufacturerof Clearﬁl S3 Bond claims that the diﬀerence between the two 10-MDP–based adhesives may lie on the ‘‘molecular dispersion technology’’ thatkeeps the homogeneity of Clearﬁl S3 Bond adhesive and prevents phase sep-aration that occurs with acetone-based all-in-one adhesives . A recentstudy showed that Clearﬁl S3 Bond is more resistant to mechanical stressthan its two-bottle predecessor , which is surprising taking into consid-eration the excellent retention rates (above 90%) of Clearﬁl SE Bondin class-V clinical studies at 2 to 3 years [53,54]. This clinical behaviorof both Clearﬁl adhesives denotes a good resistance to clinical fatigue ofadhesives containing 10-MDP.
344Table 2Recent dentin adhesivesAdhesives andmanufacturers Composition Instructions for use TypeAdheSE Ivoclar Primer: phosphoric acid acrylate, 1. Apply self-etch primer. Once the Two-step self-etch Vivadent bis-acrylic acid amide, water, cavity is thoroughly coated, brush initiators, and stabilizers for 15s. Total reaction time should Bonding component: dimethacrylate, not be shorter than 30s. hydroxy ethyl methacrylate, 2. Dry with mild airﬂow. highly dispersed silicon dioxide, 3. Apply self-etch bonding. initiators and stabilizers 4. Dry with mild airﬂow. PERDIGAO 5. Light cure for 10s.Adper Prompt 3M ESPE HEMA phosphates, HEMA, 1. Activate the L-Pop Unit Dose All-in-one self-etch, L-Pop bis-GMA, modiﬁed Dispenser to mix the adhesive. but requires mixing ˜ polyalkenoic acid, water, 2. Apply mixed adhesive to entire photo-initiator surface, rubbing in the solution with moderate ﬁnger pressure for 15s. 3. Use a gentle stream of air to thoroughly dry the adhesive into a thin ﬁlm. 4. Rewet the brush tip with adhesive and apply a second coat of adhesive to the tooth surface. The second coat does not require rubbing. 5. Use a gentle stream of air to thoroughly dry the adhesive into a thin ﬁlm. 6. Light cure for 10s.
Adper Single Bond Plus 3M ESPE HEMA, bis-GMA, DMAs, 1. Apply Scotchbond Etchant (35% Two-step etch and rinse methacrylate functional copolymer silica-thickened phosphoric acid of polyacrylic and polyitaconic gel) to tooth surface for 15s. acids, water, ethanol, nanoﬁller, 2. Rinse thoroughly for 10s. photo-initiator 3. Blot excess water using a cotton pellet or mini-sponge. Do not air dry. 4. Apply 2–3 consecutive coats of adhesive for 15s with gentle agitation using a fully saturated applicator. 5. Gently air-thin for 5s to evaporate solvent. 6. Light cure for 10s. DENTAL ADHESIONClearﬁl S3 Bond Kuraray America 10-MDP, HEMA, bis-GMA, water, 1. Thoroughly wet brush tip with All-in-one self-etch ethanol, silanated colloidal silica, Bond. Apply Bond to the tooth camphorquinone surface and leave in place for 20s. 2. Dry the entire surface suﬃciently by blowing high-pressure air for more than 5s while spreading the bond layer thinly. 3. Light cure for 10s. (continued on next page) 345
346Table 2 (continued )Adhesives andmanufacturers Composition Instructions for use TypeClearﬁl SE Bond Kuraray America Primer: 10-MDP, HEMA, hydrophilic 1. Thoroughly wet brush tip with Two-step self-etch DMA, tertiary amine, water, primer. Apply primer to the tooth photo-initiator surface and leave in place for 20s. Bonding: 10-MDP, HEMA, 2. Dry with a mild air stream to bis-GMA, hydrophilic DMA, evaporate the volatile ingredients. tertiary amine, silanated colloidal 3. Dispense the necessary amount of silica, photo-initiator Bond into second mix well. PERDIGAO 4. Apply Bond to the tooth surface. 5. After applying Bond, create a uniform ﬁlm using a gentle air ˜ stream. 6. Light cure for 10s.G-Bond GC America 4-MET, UDMA, phosphate 1. Before dispensing, shake the bottle All-in-one self-etch monomer, DMA component, fumed of G-Bond thoroughly. Replace silica ﬁller, acetone, water, bottle cap immediately after use. photo-initiator 2. Immediately apply to the prepared enamel and dentin surfaces using the microtip applicator. 3. Leave undisturbed for 10s. 4. After application, dry thoroughly using oil free air under maximum air pressure for 5s, in the presence of vacuum suction to prevent splatter of the adhesive. 5. Light cure 10s.
iBond Heraeus Kulzer UDMA, 4-MET, glutaraldehyde, 1. iBond is applied in three All-in-one self-etch acetone, water, stabilizer, consecutive layers and massaged photo-initiator into the prepared hard-tooth structure for 30s. 2. Following that, the solution is blown away with a gentle air stream. 3. Polymerize for 20s.Xeno IV Dentsply Caulk UDMA, PENTA, acetone, 1. Using the supplied disposable All-in-one self-etch polymerizeable trimethacrylate microbrush applicator tip, resin, and two polymerizeable DMA immediately apply and scrub resins, photo-initiator. surfaces with generous amounts of Xeno IV adhesive to thoroughly wet all the tooth surfaces for 15s. DENTAL ADHESION 2. Apply a second application of Xeno IV adhesive with the microbrush as above, scrubbing for 15s (20s for larger restorations). 3. Remove excess solvent by gently drying with clean, dry air from a dental syringe for at least 5s. 4. Cure Xeno IV adhesive for 10s. (continued on next page) 347
348Table 2 (continued )Adhesives andmanufacturers Composition Instructions for use TypeXP Bond Dentsply DeTrey Carboxylic acid modiﬁed 1. Etch enamel for at least 15s and Two-step etch and dimethacrylate (TCB resin), dentine for 15s or less with 36% rinse PENTA, UDMA, TEGDMA, phosphoric acid. HEMA, butylated 2. Wet all cavity surfaces uniformly benzenediol (stabilizer), with XP Bond in a disposable ethyl-4-dimethylaminobenzoate, brush. Avoid pooling. camphorquinone, functionalized 3. Leave the surface undisturbed for amorphous silica, t-butanol 20s. PERDIGAO 4. Evaporate solvent by thoroughly blowing with air from an air syringe for at least 5s. The cavity surface ˜ should have a uniform, glossy appearance. Otherwise repeat steps 2 and 4. 5. Light-cure for a minimum of 10s. Ensure uniform exposure of all cavity surfaces. 6. Immediately place the restorative material over cured XP Bond. Abbreviations: bis-GMA, bisphenol glycidyl methacrylate; DMA, dimethacrylate; HEMA, 2-hydroxyethyl methacrylate; 10-MDP, 10-methacryloyloxydecyl dihydrogenphosphate; 4-MET, 4-methacryloxyethyl trimellitic acid; PENTA, dipentaerythritol penta-acrylate phosphate; TEGDMA, triethyleneglycoldimethacrylate; UDMA, urethane dimethacrylate.
DENTAL ADHESION 349Clinical performance of all-in-one adhesives Some manufacturers of all-in-one self-etch adhesives do not recommendenamel pre-etching, while other manufacturers recommend phosphoric-acidetching of unground enamel. One would argue that additional enamel bondstrength is always required to prevent marginal gaps and leakage. In a clin-ical setting, the adhesive is extended past the boundaries of the preparation,forming composite ﬂashes. Bonding to this uninstrumented surface isneeded to resist potential staining. The manufacturer of Xeno IV (Dentsply)recommends beveling the enamel margins for all procedures, which may bediﬃcult to achieve in the cervical margin of class-II preparations. The man-ufacturers of Adper Prompt L-Pop (3M ESPE) and iBond (Heraeus Kulzer)do not recommend a separate enamel-etching step. The manufacturerof Clearﬁl S3 Bond (Kuraray) recommends phosphoric-acid etching ofunground enamel. Pre-etching may improve bonding to uninstrumentedsurfaces for all mild all-in-one adhesives, especially in areas where an adhe-sive ﬂash formed during insertion. When enamel is etched separately, bondstrengths increase signiﬁcantly for self-etch adhesives [52,55]. However, ifetching is extended to dentin, bonding may be compromised . The enamel bond strengths of aggressive self-etch adhesives are usuallyhigher than those of other self-etch adhesives , which may have to dowith the relatively low pH compared with other less acidic adhesives (seeTable 1). A recent morphological scanning electron microscopy study re-ported that the etching pattern on Adper Prompt, the bottle version of AdperPrompt L-Pop, is similar to that of phosphoric acid . Other all-in-oneadhesives, such as G-Bond (GC America) and iBond (Heraeus Kulzer), donot result in any discernible etching pattern or minimal exposure of crystallitesin sporadic areas of unground enamel. On ground enamel, these adhesives re-sult in islands of superﬁcially dissolved enamel within areas without any signof enamel dissolution (Fig. 15). One of the ﬁrst clinical signs that a compositeFig. 15. (A) Field emission scanning electron micrograph of enamel treated with iBond (Her-aeus Kulzer) after roughening the enamel with a diamond bur for 5 seconds. The adhesivewas removed with acetone. (B) Enamel etched with 38% phosphoric acid (Pulpdent) for 15seconds.
350 ˜ PERDIGAOrestoration is prone to failure is its early marginal staining. In fact, iBond isunable to penetrate the enamel smear layer , which explains why it is notvery eﬀective when applied on ground enamel. The almost inexistent etchingpattern of iBond (an adhesive based on 4-methacryloxyethyl trimellitic acid(4-MET)) may have been responsible for massive marginal failure in a poste-rior composite clinical study at 1 year . The all-in-one adhesive iBond re-sulted in statistically worse marginal staining than any of the other adhesivesused in this study. Two other adhesives, a 10-MDP–based all-in-one adhesive(Clearﬁl S3 Bond) and a self-etch adhesive based on polyalkenoic acid copol-ymer and hydroxyethyl-methacrylate (Adper Prompt L-Pop) resulted ina slightly lower percentage of excellent margins than the etch-and-rinse adhe-sive One-Step Plus, but these diﬀerences were not signiﬁcant. At 1 year, the res-torations inserted with iBond showed a dark orange aspect in most of therestorations, which was already evident at 6 months (Figs. 16 and 17). Thechange in color of the restoration might have been a result of the degradationof the adhesive itself, not that of the composite material, as the other adhesivesdid not result in such catastrophic results. This color change of the 4-MET–based all-in-one adhesive may be a result of its rapid hydrolysis, which is tem-perature-dependent and occurs as early as at 1 month, when specimens arestored at 25 C to 37 C . Marginal adaptation is another parameter for which some self-etch adhe-sives result in unacceptable clinical results, which means they have a deﬁcientenamel bonding ability. This bonding inability has been observed in labora-tory studies as some all-in-one self-etch adhesives fail prematurely, with pre-testing failures in the range of 50% . Another study found 50% to 66%of pretesting failures with iBond with and without 20,000 cycles of thermalfatigue . When the prevailing failure mode is adhesive, the bondstrengths are generally low, while cohesive failures are more often associatedwith high bond strengths . Several investigators have reported very lowbond strengths with iBond when applied as per manufacturer’s directions[37,61–63]. Clinically, iBond has resulted in more marginal staining thanan etch-and-rinse adhesive in a class-V study , which corroborates theFig. 16. Tooth #30 (left) preoperatively and (right) 1 year after being restored with the etch-and-rinse adhesive One-Step Plus (Bisco Inc.).
DENTAL ADHESION 351Fig. 17. Tooth #19 (left) preoperatively and (right) 1 year after being restored with the all-in-one self-etch adhesive iBond (Heraeus Kulzer) (same patient as in Fig. 15).poor marginal staining observed in the 1-year posterior composite clinicalstudy . In that class-V study , iBond was compared with Gluma SolidBond (Heraeus Kulzer), an etch-and-rinse adhesive, at 18 months. Otherstudies have also reported severe enamel microleakage in vitro, especiallywith thermal stresses with iBond [39,40], which explains the high percentageof marginal openings found clinically. Only 2 out of 27 iBond restorationswere rated Alfa for marginal adaptation at 1 year . According to the American Dental Association (ADA) guidelines forenamel and dentin adhesives, the cumulative incidence of clinical failures ineach of two independent studies must be less than 10% to obtain full accep-tance at 18 months . While the enamel bonding ability of mild all-in-oneadhesives may be jeopardized by thermal and mechanical fatigue, more ag-gressive all-in-one adhesives have resulted in acceptable clinical behavior[57,66]. At 18-months, 7% of the class-V restorations placed with AdperPrompt were lost versus none of the restorations inserted with Single Bond(3M ESPE), an etch-and-rinse adhesive . The restorations bonded withSingle Bond had slightly better marginal adaptation and marginal discolor-ation, but not statistically better. In spite of a slightly poorer clinical behaviorat 18 months in class-V noncarious lesions, all-in-one adhesives like AdperPrompt have demonstrated lower bond strength to both enamel and dentinthan one-bottle etch-and-rinse systems, such as Single-Bond [15,28,67]. In a posterior composite clinical study , marginal staining with AdperPrompt L-Pop at 1 year was not signiﬁcantly diﬀerent from baseline, but theP value was close to signiﬁcance (P ¼ .06). Marginal adaptation at 1 yearwas signiﬁcantly worse than at baseline (P!.0001), as 18 out of 29 restora-tions were rated Bravo and 2 restorations were rated Charlie. Postoperativesensitivity to air at 1 year improved signiﬁcantly for Adper Prompt L-Pop ascompared with the preoperative values (P!.016). All 7 restorations thatwere sensitive to air preoperatively were not sensitive at 1 year. While the aggressiveness (acidity) of the self-etch solution is important todetermine the interaction depth of the restorative material with enamel, thechemical attributes of all-in-one adhesive are also important. Clinical studies
352 ˜ PERDIGAOwith Prompt L-Pop, the predecessor of Adper Prompt, in cervical lesions re-sulted in a high failure rate [68,69]. The most crucial diﬀerence between thetwo versions is the presence of the polyalkenoic-acid copolymer in the latestversions (Adper Prompt and Adper Prompt L-Pop). This polyalkenoate-based component was ﬁrst introduced in a resin-modiﬁed glass ionomer ma-terial (Vitrebond, 3M ESPE) and subsequently used in other formulations,including the adhesive systems (Scotchbond Multi-Purpose Primer and Sin-gle Bond). The polyalkenoate salt has been claimed to provide water stabil-ity to the adhesive system by a dynamic potential of breaking and renewingthe bonding between the carboxyl groups and calcium, forming a stress-relaxation zone at the bonded interface .Etch-and-rinse adhesives: Are they the benchmark for other adhesives? Etch-and-rinse adhesives result in high enamel and dentin bond strengths.The enamel-etching pattern and the penetration into the dentinal substrate re-inforce the idea that etch-and-rinse adhesives are still the benchmark for otheradhesives when it comes to laboratory performance [26,27,47]. However, thereare still concerns regarding the degree of inﬁltration of the etched dentin bysome etch-and-rinse adhesives, such the ethanol- and water-based SingleBond, the unﬁlled version of Adper Single Bond Plus [71–73]. In spite of thehigh retention rate in clinical studies, reports have indicated that the bondsformed with Single Bond may undergo degradation in vivo at 1 year . Acetone-based etch-and-rinse adhesives are more technique-sensitivethan adhesives containing ethanol or water [74,75]. The clinical behaviorof acetone-based etch-and-rinse adhesives may be determined by variationsin the respective application technique, namely the amount of moisture leftafter rinsing the etchant and the amount of adhesive applied in the prepara-tion . One-Step Plus is the ﬁlled version of the acetone-based etch-and-rinse adhesive One-Step. Dentin bond strengths do not improve when theﬁlled version is used [52,75]. Clinical studies using One-Step in class-V le-sions have resulted in a wide variety of retention rates. One study found a re-tention rate of 75% at 3 years, while another study reported a 56% retentionrate at 18 months [77,78]. Van Dijken  reported a 51% retention rate at3 years, with higher failure rates in cervical lesions with sclerotic dentin. Thislow retention rate reported in some studies is not in agreement with the highdentin and enamel bond strengths found in other studies [80,81]. For multi-bottle etch-and-rinse adhesives, 5 full papers and 11 abstractswere published from 1998 to 2004 . In 81% of the studies, multi-bottleetch-and-rinse adhesives fulﬁlled the full acceptance ADA guidelines (18months), with an average annual failure rate of 4.8% . With regard toone-bottle etch-and-rinse adhesives, 15 full papers and 17 abstracts ap-peared in the literature in the same period . The clinical performanceof multibottle etch-and-rinse adhesives was better than that of one-bottle
DENTAL ADHESION 353etch-and-rinse adhesives, as only 51% fulﬁlled the full acceptance ADAguidelines (18 months) . Even though dental adhesives have been avail-able over several generations with an array of new materials being launchedevery year, clinical studies are not abundant in the literature. Several reasonsmay account for the discrepancy: ﬁrst, the time constraints associated withsetting up and running a clinical study with the respective periodic recalls;second, a generalized scarcity of industrial and independent funding forthis type of applied research; and third, the frequent practice among manu-facturers to launch a new version of a speciﬁc adhesive even before theprevious one has been fully tested. As a result of all these limitations, re-searchers and clinicians still rely on data from laboratory studies to predictthe behavior of adhesive materials.Summary Numerous simpliﬁed adhesives have been introduced to the dental mar-ket within the last few years, sometimes without comprehensive testing tovalidate the performance claimed by the respective manufacturers. Mildself-etch adhesives are unable to etch enamel to provide adequate retentionfor bonded restorations. Although high early resin–dentin bond strengthvalues can be achieved with some self-etch adhesives, their resistance to ther-mal and mechanical stresses over time is disappointing. In light of the cur-rent drawbacks attributed to all-in-one self-etch adhesives, etch-and-rinseadhesives are still the benchmark for dental adhesion in routine clinical use.Acknowledgments The author gives special thanks to Drs. S. Duarte, G. Gomes, andM. Lopes for help preparing the scanning electron microscopy and trans-mission electron microscopy specimens.References Buonocore MG. A simple method of increasing the adhesion of acrylic ﬁlling materials to enamel surfaces. J Dent Res 1955;34:849–53. Swift EJ, Perdigao J, Heymann HO. Bonding to enamel and dentin: a brief story and state of ˜ the art. Quintessence Int 1995;26:95–110. Baier RE. Principles of adhesion. Oper Dent Suppl 1992;5:1–9. Pashley DH. The eﬀects of acid etching on the pulpodentin complex. Oper Dent 1992;17: 229–42. Asmussen E, Uno S. Adhesion of restorative resin to dentin: chemical and physicochemical aspects. Oper Dent Suppl 1992;5:68–74. Bowen RL, Eick JD, Henderson DA, et al. Smear layer: removal and bonding consider- ations. Oper Dent Suppl 1984;3:30–4. Eick JD, Cobb CM, Chapell RP, et al. The dentinal surface: its inﬂuence on dentinal adhe- sion. Part I. Quintessence Int 1991;22:967–77.
354 ˜ PERDIGAO  Suzuki T, Finger WJ. Dentin adhesives: site of dentin vs. bonding of composite resins. Dent Mater 1988;4:379–83.  Gwinnett AJ. Smear layer: morphological considerations. Oper Dent Suppl 1984;3:3–12. Perdigao J. Dentin bonding as function of dentin structure. Dent Clin North Am 2002;46: ˜ 1–25. Nakabayashi N, Kojima K, Masuhara E. The promotion of adhesion by the inﬁltration of monomers into tooth substrates. J Biomed Mater Res 1982;16:265–73. Brannstrom M, Nordenvall KJ. The eﬀect of acid etching on enamel, dentin, and the inner ¨ ¨ surface of the resin restoration: a scanning electron microscopic investigation. J Dent Res 1977;56:917–23. Davidson CL, de Gee AJ, Feilzer A. The competition between the composite-dentin bond strength and the polymerization contraction stress. J Dent Res 1984;63:1396–9. Perdigao J, Lambrechts P, Van Meerbeek B, et al. The interaction of adhesive systems with ˜ human dentin. Am J Dent 1996;9:167–73. Van Meerbeek B, De Munck J, Yoshida Y, et al. Buonocore memorial lecture. Adhe- sion to enamel and dentin: current status and future challenges. Oper Dent 2003;28: 215–35. Pashley DH, Tay FR. Aggressiveness of contemporary self-etching adhesives. Part II: etching eﬀects on unground enamel. Dent Mater 2001;17:430–44. Van Meerbeek B, Perdigao J, Lambrechts P, et al. The clinical performance of dentin adhesives. J Dent 1998;26:1–20. Tay FR, Pashley DH. Aggressiveness of contemporary self-etching systems. I: depth of penetration beyond smear layers. Dent Mater 2001;17:296–308. Perdigao J, Gomes G, Lopes MM. The inﬂuence of conditioning time on enamel adhesion. ˜ Quintessence Int 2006;37:41–7. Nishitani Y, Yoshiyama M, Wadgaonkar B, et al. Activation of gelatinolytic activity in dentin by self-etching adhesives. Eur J Oral Sci 2006;114:160–6. Van Landuyt KL, De Munck J, Snauwaert J, et al. Monomer-solvent phase separation in one-step self-etch adhesives. J Dent Res 2005;84:183–8. Carvalho RM, Stefano Chersoni S, Frankenberger R, et al. A challenge to the conventional wisdom that simultaneous etching and resin inﬁltration always occurs in self-etch adhesives. Biomaterials 2005;26:1035–42. Perdigao J, Geraldeli S. Bonding characteristics of self-etching adhesives to intact vs. ˜ prepared enamel. J Esthet Restor Dent 2003;15:32–42. Kanemura N, Sano H, Tagami J. Tensile bond strength to and SEM evaluation of ground and intact enamel surfaces. J Dent 1999;27:523–30. Van Meerbeek B, De Munck J, Mattar D, et al. Microtensile bond strength of an etchrinse and self-etch adhesive to enamel and dentin as a function of surface treatment. Oper Dent 2003;28:647–60. Goracci C, Sadek FT, Monticelli F, et al. Microtensile bond strength of self-etching adhesives to enamel and dentin. J Adhes Dent 2004;6:313–8. Perdigao J, Gomes G, Duarte S Jr, et al. Enamel bond strengths of pairs of adhesives from ˜ the same manufacturer. Oper Dent 2005;30:492–9. Armstrong SR, Vargas MA, Fang Q, et al. Microtensile bond strength of a total-etch 3-step, total-etch 2-step, self-etch 2-step, and a self-etch 1-step dentin bonding system through 15-month water storage. J Adhes Dent 2003;5:47–56. Tay FR, Kwong S-M, Itthagarun A, et al. Bonding of a self-etching primer to non-carious cervical sclerotic dentin: interfacial ultrastructure and microtensile bond strength evalua- tion. J Adhes Dent 2000;2:9–28. De Munck J, Vargas M, Iracki J, et al. One-day bonding eﬀectiveness of new self-etch adhesives to bur-cut enamel and dentin. Oper Dent 2005;30:39–49. Tay FR, Pashley DH, Suh BI, et al. Single-step adhesives are permeable membranes. J Dent 2002;30:371–82.
DENTAL ADHESION 355 Tay FR, Pashley DH. Water treeingda potential mechanism for degradation of dentin adhesives. Am J Dent 2003;16:6–12. De Munck J, Van Landuyt K, Coutinho E, et al. Micro-tensile bond strength of adhesives bonded to class-I cavity-bottom dentin after thermo-cycling. Dent Mater 2005;21:999–1007. Frankenberger R, Tay FR. Self-etch vs etch-and-rinse adhesives: Eﬀect of thermo-mechan- ical fatigue loading on marginal quality of bonded resin composite restorations. Dent Mater 2005;21:397–412. Bergenholtz G. Evidence for bacterial causation of adverse pulpal responses in resin-based restorations. Crit Rev Oral Biol Med 2000;11:467–80. Sensi LG, Lopes GC, Monteiro S Jr, et al. Dentin bond strength of self-etching primers/ adhesives. Oper Dent 2005;30:63–8. Ito S, Tay F, Hashimoto M, et al. Eﬀects of multiple coatings of two all-in-one adhesives on dentin bonding. J Adhes Dent 2005;7:133–41. Frankenberger R, Perdigao J, Rosa BT, et al. ‘‘No-bottle’’ vs ‘‘multi-bottle’’ dentin adhe- sivesda microtensile bond strength and morphological study. Dent Mater 2001;17:373–80. Brackett MG, Brackett WW, Haisch LD. Microleakage of Class V resin composites placed using self-etching resins: eﬀect of prior enamel etching. Quintessence Int 2006;37:109–13. Kubo S, Yokota H, Yokota H, et al. Microleakage of cervical composites restored with one- step self-etch systems [abstract]. J Dent Res 2005;84(Spec Iss A). Pashley DH, Ciucchi B, Sano H, et al. Permeability of dentin to adhesive agents. Quintes- sence Int 1993;24:618–31. De Munck J, Van Meerbeek B, Yoshida Y, et al. Four-year water degradation of total-etch adhesives bonded to dentin. J Dent Res 2003;82:136–40. Hashimoto M, Tay FR, Ohno H, et al. SEM and TEM analysis of water degradation of human dentinal collagen. J Biomed Mater Res Part: B Appl Biomater 2003;66:289–98. Carrilho MR, Carvalho RM, Tay FR, et al. Durability of resin-dentin bonds related to water and oil storage. Am J Dent 2005;18:315–9. Hashimoto M, Ohno H, Sano H, et al. Micromorphological changes in resin-dentin bonds after 1 year of water storage. J Biomed Mater Res Part: B Appl Biomater 2002;63:306–11. Santerre JP, Shajii L, Leung BW. Relation of dental composite formulations to their degra- dation and the release of hydrolyzed polymeric-resin-derived products. Crit Rev Oral Biol Med 2001;12:136–51. Spreaﬁco D, Semeraro S, Mezzanzanica D, et al. The eﬀect of the air-blowing step on the technique sensitivity of four diﬀerent adhesive systems. J Dent 2006;34:237–44. Tay FR, King NM, Chan KM, et al. How can nanoleakage occur in self-etching adhesive systems that demineralize and inﬁltrate simultaneously? J Adhes Dent 2002;4:255–69. Tay FR, Lai CN, Chersoni S, et al. Osmotic blistering in enamel bonded with one-step self- etch adhesives. J Dent Res 2004;83:290–5. Ito S, Hashimoto M, Wadgaonkar B, et al. Eﬀects of resin hydrophilicity on water sorption and changes in modulus of elasticity. Biomaterials 2005;26:6449–59. Hoﬀmann M, Eppinger R, Kastrani A, et al. FTIR conversion analysis of all-in-one adhesives using diﬀerent methods [abstract]. J Dent Res 2006;85(spec issue A). Can Say E, Nakajima M, Senawongse P, et al. Microtensile bond strength of a ﬁlled vs un- ﬁlled adhesive to dentin using self-etch and total-etch technique. J Dent 2006;34:283–91. Turkun SL. Clinical evaluation of a self-etching and an one bottle adhesive at two years. ¨ ¨ J Dent 2003;31:527–34. Van Meerbeek B, Kanumilli P, De Munck J, et al. A randomized controlled study evaluating the eﬀectiveness of a two-step self-etch adhesive with and without selective phosphoric-acid etching of enamel. Dent Mater 2005;21:375–83. Miguez PA, Castro PS, Nunes MF, et al. Eﬀect of acid-etching on the enamel bond of two self-etching systems. J Adhes Dent 2003;5:107–12. Di Hipolito V, de Goes MF, Carrilho MR, et al. SEM evaluation of contemporary self-etch- ing primers applied to ground and unground enamel. J Adhes Dent 2005;7:203–11.
356 ˜ PERDIGAO Perdigao J, Dutra-Correa M, Castilhos N, et al. One-year clinical performance of self-etch ˜ ˆ adhesives in posterior restorations. Am J Dent, in press. Nishiyama N, Tay FR, Fujita K, et al. Hydrolysis of functional monomers in a single-bottle self-etching primerdcorrelation of 13C NMR and TEM ﬁndings. J Dent Res 2006;85:422–6. Perdigao J, Gomes G, Gondo R, et al. In vitro bonding performance of all-in-one adhesives. ˜ Part Idmicrotensile bond strengths. J Adhes Dent 2006;8:367–73. Pereira PN, Okuda M, Sano H, et al. Eﬀect of intrinsic wetness and regional diﬀerence on dentin bond strength. Dent Mater 1999;15:46–53. Atash R, Van den Abbeele A. Bond strengths of eight contemporary adhesives to enamel and to dentine: an in vitro study on bovine primary teeth. Int J Paediatr Dent 2005;15:264–73. Soderholm KJ, Guelmann M, Bimstein E. Shear bond strength of one 4th and two 7th gen- ¨ eration bonding agents when used by operators with diﬀerent bonding experience. J Adhes Dent 2005;7:57–64. Van Landuyt KL, Peumans M, De Munck J, et al. Extension of a one-step self-etch adhesive into a multi-step adhesive. Dent Mater 2006;22:533–44. Ritter AV, Heymann H, Pereira P, et al. Clinical evaluation of an all-in-one self-etching dental adhesive [abstract]. J Dent Res 2005;84(Spec Iss A). American Dental Association Council of Scientiﬁc Aﬀairs. Acceptance program guidelines dentin and enamel adhesive materials. Available at: http://www.ada.org/ada/seal/standards/ guide_materials_adhesive.pdf. Accessed February 10, 2007. Bittencourt DD, Ezecelevski IG, Reis A, et al. An 18-months’ evaluation of self-etch and etch rinse adhesive in non-carious cervical lesions. Acta Odontol Scand 2005;63:173–8. Inoue S, Vargas MA, Abe Y, et al. Microtensile bond strength of eleven contemporary adhesives to enamel. Am J Dent 2003;16:329–34. Brackett WW, Covey DA, St Germain HA Jr. One-year clinical performance of a self-etch- ing adhesive in Class V resin composites cured by two methods. Oper Dent 2002;27:218–22. van Dijken JWV. Durability of three simpliﬁed adhesive systems in Class V non-carious cervical dentin lesions. Am J Dent 2004;17:27–32. Eliades GC. Dentine bonding systems. In: Vanherle G, Degrange M, Willems G, editors. State of the art on direct posterior ﬁlling materials and dentine bonding. Leuven (Belgium): Van der Poorten; 1993. p. 49–74. Wang Y, Spencer P, Hager C, et al. Comparison of interfacial characteristics of adhesive bonding to superﬁcial versus deep dentine using SEM and staining techniques. J Dent 2006;34:26–34. Wang Y, Spencer P. Evaluation of the interface between one-bottle adhesive systems and dentin by Goldner’s trichrome. Am J Dent 2005;18:66–72. Koshiro K, Inoue S, Tanaka T, et al. In vivo degradation of resin–dentin bonds produced by a self-etch vs. a total-etch adhesive system. Eur J Oral Sci 2004;112:368–75. Tay FR, Gwinnett JA, Wei SH. Micromorphological spectrum from overdrying to overwet- ting acid-conditioned dentin in water-free acetone-based, single-bottle primer/adhesives. Dent Mater 1996;12:236–44. Lee YK, Pinzon LM, O’Keefe KL, et al. Eﬀect of ﬁller addition on the bonding parameters of dentin bonding adhesives bonded to human dentin. Am J Dent 2006;19:23–7. Platt JA, Almeida J, Gozalez-Cabezas C, et al. The eﬀect of double adhesive application on the shear bond strength to dentin of compomers using three one-bottle adhesive systems. Oper Dent 2001;26:313–7. Tyas MJ, Burrow MF. Three-year clinical evaluation of One-Step in non-carious cervical le- sions. Am J Dent 2002;15:309–11. Brackett WW, Brackett MG, Dib A, et al. Eighteen-month clinical performance of a self- etching primer in unprepared class V resin restorations. Oper Dent 2005;30:424–9. Van Dijken JWV. Clinical evaluation of three adhesive systems in class V non-carious lesions. Dent Mater 2000;16:285–91.
DENTAL ADHESION 357 Loguerico AD, Uceda-Gomez N, Carrilho MR, et al. Inﬂuence of specimen size and regional variation on long-term resin-dentin bond strength. Dent Mater 2005;21:224–31. Reis A, Loguercio AD, Azevedo CL, et al. Moisture spectrum of demineralized dentin for adhesive systems with diﬀerent solvent bases. J Adhes Dent 2003;5:183–92. Peumans M, Kanumilli P, De Munck J, et al. Clinical eﬀectiveness of contemporary adhe- sives: a systematic review of current clinical trials. Dent Mater 2005;21:864–81.